Polymerization pattern characterization within a resin-based composite cured using different curing units at two distances
- 23 Downloads
To investigate the relationship of the irradiance-beam-profile areas from six different light-curing units (LCUs) with the degree of conversion (DC), microhardness (KH), and cross-link density (CLD) throughout a resin-based composite (RBC) cured at two clinically relevant distances, and to explore the correlations among them.
Materials and methods
A mapping approach was used to measure DC using micro-Raman spectroscopy, KH using a Knoop indentor on a hardness tester, and %KH reduction after ethanol exposure, as an indicator for CLD within a nano-hybrid RBC increment (n = 3) at various depths. These sample composites were cured from two distances while maintaining the radiant exposure, using six different light-curing units: one quartz-tungsten-halogen; two single and three multiple-emission-peak light-emitting-diode units. Irradiance beam profiles were generated for each LCU at both distances, and localized irradiance values were calculated. Points across each depth were analyzed using repeated measures ANOVA. Correlations across multiple specimen locations and associations between beam uniformity corresponding with polymerization measurements were calculated using linear mixed models and Pearson correlation coefficients.
Significant non-uniform polymerization patterns occurred within the specimens at various locations and depths. At 2-mm curing distance, the localized DC = 52.7–76.8%, KH = 39.0–66.7 kg/mm2, and %KH reduction = 26.7–57.9%. At 8-mm curing distance, the localized DC = 50.4–78.6%, KH = 40.3–73.7 kg/mm2, and %KH reduction = 28.2–56.8%. The localized irradiance values were weakly correlated with the corresponding DC, KH, and %KH reduction, with only a few significant correlations (p < 0.05).
Although significant differences were observed at each depth within the specimens, the localized irradiance values for all LCUs did not reflect the polymerization pattern and did not seem to have a major influence on polymerization patterns within the RBC, regardless of the curing distance.
Commonly used LCUs do not produce uniform polymerization regardless of the curing distance, which may contribute to the risk of RBC fracture.
KeywordsDegree of conversion Microhardness Cross-link density Resin composite Beam profile Light-curing unit
The work is part of the PhD dissertation for Dr. A. O. Al-Zain. The scholarship support from King Abdulaziz University, Jeddah, Saudi Arabia, and the technical assistance received from UITS/PTI Advanced Visualization Lab at Indiana University are acknowledged.
Compliance with ethical standards
Conflict of interest
The authors declare that they have no conflict of interest.
This article does not contain any studies with human participants or animals performed by any of the authors.
For this type of study, formal consent is not required.
- 12.Selig D, Haenel T, Hausnerova B, Moeginger B, Labrie D, Sullivan B, Price RB (2015) Examining exposure reciprocity in a resin based composite using high irradiance levels and real-time degree of conversion values. Dent Mater 31:583–593. https://doi.org/10.1016/j.dental.2015.02.010 CrossRefGoogle Scholar
- 17.Yap AU, Soh MS, Han TT, Siow KS (2004) Influence of curing lights and modes on cross-link density of dental composites. Oper Dent 29:410–415Google Scholar
- 20.Rueggeberg FA, Giannini M, Arrais CAG, Price RBT (2017) Light curing in dentistry and clinical implications: a literature review. Braz Oral Res 31:e61. https://doi.org/10.1590/1807-3107BOR-2017.vol31.0061 CrossRefGoogle Scholar
- 29.Price RB, Labrie D, Whalen JM, Felix CM (2011) Effect of distance on irradiance and beam homogeneity from 4 light-emitting diode curing units. J Can Dent Assoc 77:b9Google Scholar
- 33.Mousavinasab SM, Meyers I (2011) Comparison of depth of cure, hardness and heat generation of LED and high intensity QTH light sources. Eur J Dent 5:299–304Google Scholar
- 36.Vasudeva G (2009) Monomer systems for dental composites and their future: a review. J Calif Dent Assoc 37:389–398Google Scholar
- 40.Sampaio CS, Atria PJ, Rueggeberg FA, Yamaguchi S, Giannini M, Coelho PG, Hirata R, Puppin-Rontani RM (2017) Effect of blue and violet light on polymerization shrinkage vectors of a CQ/TPO-containing composite. Dent Mater 33:796–804. https://doi.org/10.1016/j.dental.2017.04.010 CrossRefGoogle Scholar
- 43.ISO (2007) 10650-2:2007 dentistry-powered polymerizationactivators: part 2: light-emitting diode (LED) lamps. Geneva,Switzerland: International Standards Organization.:7Google Scholar